On October 23rd, 2014, we updated our
By continuing to use LinkedIn’s SlideShare service, you agree to the revised terms, so please take a few minutes to review them.
COMPOSITE MATERIAL FIRE FIGHTING Presented to: International Aircraft Materials Fire Test Working Group Renton, Washington, USA Presented By: John C. Hode SRA International Date: Wednesday, March 3, 2009
Revised thermocouple position simulates aircraft skin with insulation backing
Tracings no longer showed any lags
Hidden Areas cont.
10 minute exposures reliably reached at or above 1200°F (654°C). Average 1367.2°F (741.7°C)
Maximum 1425.6°F (774.2°C)
Minimum 1282.8°F (694.8°C)
1 or 3 minute exposures were on average about 200°F (93.3°C) above the measured panel temperatures. Average 828.1°F (442.3°C)
Maximum 1293.2°F (700.6°C)
Minimum 619°F (326.1°C)
Maximum temperatures unchanged due to revised thermocouple position.
Test 4 panel shown
7 tests suffered sudden mechanical failures
Failures occurred in 30 seconds on average
Mechanical Failures cont.
Quintiere  attributed swelling to vaporization of epoxy, thereby causing internal pressure.
All panels in these tests produced heavy out-flow of smoke from the edges, not the panel face, and swelled to varying degrees.
In these tests, panel edges were sometimes tightly fit into back Kaowool board.
May have restricted outflow of smoke and off-gassing.
It was observed during video review that in one test heavy smoking from the edge markedly reduced, when the failure occurred a surge of heavy smoke erupted from the failure site.
The mechanical failures may have been due to over-pressurization but this was not further explored in this series of tests.
All panels emitted smoke.
Onset of smoke production ranged 111°F (44°C) to 392°F (202°C) by thermocouple measurement.
FLIR temperatures at the onset of smoke production ranged 139°F (60°C) to 621°F (330°C).
Definitively, smoke did not occur under 100°F (38°C).
Firefighters could use smoke production as an indicator of continued combustion but an imprecise indicator of temperature. Where smoking persists temperatures may still be above 300°F (150°C), and should be assumed so unless proven otherwise.
Heavy smoke from the backside was sometimes ignited by the front side flame. This was clearly observed during the video review.
Here, the ignition of back-side off-gassing happened after the burner was turned off.
From Test 18 video
Rear Flashover cont.
Two tests suffered mechanical failures at the bottom edge that allowed high heat to contact and ignite smoke emitting from bottom edge.
Ignition of edge involved part of the panel face which evolved into flashover of the backside.
Test 4 Flashover Test 21 Flashover
Some amount of flame continued after burner removal in every test.
Duration of the flame; as little as 1 second or as much as 3 minutes.
Test 6 & 16; flickers of flame could be seen inside the panel, behind delaminated outer plies.
Median flame extinction times were;
75 seconds for 1 minute exposures
50 seconds for 3 minute exposures
25 seconds for 5 minute exposures
17 seconds for 10 minute exposures
This, and panel weight after exposure, reinforce the theory that duration of flaming combustion is a factor of epoxy content.
During review of the video for the first 12 tests, areas of smoldering were observed.
Color camera view after test 12 was tightened so that occurrences of smoldering could be seem more clearly.
14 of the 23 total tests had at least one occurrence of smoldering. Some tests had two or more separate occurrences. Each separate location was considered an occurrence.
Most occurrences were in the corners. Test 16, a 1 minute exposure, showed smoldering in the center of the panel.
Post-Exposure Smoldering cont.
Corner temperatures at onset and extinction of smoldering were compared to panel temperatures, where sufficient data was available.
Corner temperatures reduced 30% from onset to extinction while the panel temperature reduced 50%.
Introduction of a Fan
A small floor fan was used to simulate airfield wind conditions.
Fan produced 7-8 mph of wind speed at a 4 foot distance.
Used in 5 tests.
Fan intensified smoldering in some cases but blew-out flames. However, there were cases where backside flames were promoted by increased oxygen flow.
In other instances, wind promoted smoldering where it did not initially exist.
Test 18, smoldering initiated 90 seconds after removal of the burner.
Other tests experienced an onset of smoldering up to 2 minutes, 33 seconds after fire exposure.
10 minute exposures had more and longer occurrences of smoldering.
Re-ignition noted in three tests.
Two of those tests the re-ignition was not significant. One was just a flicker, the other was likely continued flaming.
Test 19 (10 min, with fan) ignited 64 seconds after burner removal and intermittently persisted for almost 3 minutes.
Wind seems to promote flaming and re-ignition in areas where the flow of oxygen is increased but protected from the wind, which would otherwise blow-out the flame.
Other Test Configurations
Tests 22 and 23
The panel was cut into 4 pieces and stacked with ¾ inch (76.2mm) spaces between.
Thermocouples placed on top surface of each layer.
Exposure time; 1 minute.
Other Test Configurations cont.
Measured temperatures in the vicinity of 1750°F (962°C).
As smoldering continued, plies could be seen to drop onto layers below.
When layers were taken apart for disposal they had virtually no structural strength.
Wind (in Test 22) caused smoldering to last 52 seconds longer.
Phase II testing test plan being written.
Gas fired line burner planned for fire source. Burner will be 2 ft (60.96 cm) wide, flame height could be as much as 6 feet (182.88 cm).
Thermocouple array or similar will be used to characterize the flame. Replication of aviation fuel pool fire temperatures still the objective.
Sample panels will be 4 ft wide by 6 ft tall to avoid edge effects.
Standard aircraft insulation will be included to see if certain results noted here can be replicated.
Agent application planned to be remotely controlled and from a fixed device to limit variability of human application.
Straight stream and cone pattern flows considered.
Simple geometries, (T-type form) mentioned in October, are not part of Phase II plan. However, may be the focus of a separate study, but nothing planned yet.
Quintiere, J.G., Walters, R.N., Crowley, S., "Flammability Properties of Aircraft Carbon-Fiber Structural Composite," FAA report DOT/FAA/AR-07/57, October 7, 2008.